# Fabrication and Antibacterial Effects of Polycarbonate/Leaf Extract Based Thin Films

Authors: R. Mahendran; D. Sridharan; C. Arunmozhidevan; T. A. Selvakumar; P. Rajasekar
Journal: Journal of Materials
 (2016)

---

## Abstract

We have reported the preparation and antibacterial activities of leaf extract incorporated polycarbonate thin films to improve the antibacterial characteristics of host polycarbonates (PCs). Crude extracts ofAzadirachta indica, Psidium guajava, Acalypha indica, Andrographis paniculata, andOcimum sanctum were prepared by maceration using Dimethylformamide as solvent. The leaf extracts (LE) were incorporated into the PC matrix by solution blending method, and the thin films were fabricated by Thermally Induced Phase Separation (TIPS) technique. The antibacterial activities of the as-prepared films were evaluated againstE. coli andS. aureus by disk diffusion method. The inhibitory effects of the PC/LE films are higher forS. aureus than theE. coli, but pristine PC film did not exhibit any remarkable antibacterial characteristics. Further, the model fruit (Prunus) studies revealed that the PC/LE films retained the freshness of the fruits for more than 11 days. This study demonstrates that the PC/LE films have excellent antibacterial activities; thus, the films could be promising candidate for active antibacterial packaging applications.


---

## Body

## 1. Introduction

Bacterial growth on food surface is the main cause of spoilage of the foods. In order to control undesirable bacterial activities on foods, antibacterial packaging films are being utilized to keep the food safe. The antibacterial materials inhibit/reduce the ability of bacterial colonies to grow on the surface of the food. Generally, the antibacterial materials are blended/immobilized/coated on the packaging materials to prolong shelf-life, sensory properties, and freshness of the food [1]. Furthermore, antibacterial materials protect the food from pathogens, oxygen, moisture, and dust. Generally, antibacterial materials have been fabricated by incorporating biologically active compounds such as antioxidants and flavoring agents into matrix/coating of the packaging material [2, 3], which reduce the growth of bacteria.Conventionally, the metal nanoparticles are being impregnated into the polymer matrix for enhancing their antibacterial activities; however, they have certain drawbacks such as high cost, toxicity, harmfulness, and problems in disposal of the wastes [4, 5]. In order to overcome these difficulties, ecofriendly antibacterial materials such as medicinal leaf extract are used for destroying Gram-positive and Gram-negative bacteria [6]. The leaf extracts are in liquid form, which protect their commercial applications in active packaging materials. This major drawback could be overcome by incorporating the leaf extract into the polymer matrix for the fabrication of films, which can protect the food and beverages from the bacterial attack. Generally, most of the leaf extracts have rich content of tannins, terpenoids, alkaloids, flavonoids, glycosides, and polyphenols, which was clearly identified as theirin vitro antibacterial activities.The biodegradable polymers like cellulosic polymers have been utilized for the fabrication of antibacterial packaging films; however, their water sensitivity, poor interfacial adhesion, and low melting point reduce their potential applications. In order to overcome these drawbacks, polycarbonate (PC) based thin films have been used for food packaging, due to their hydrophobic nature, durability, dimensional stability, light weight, excellent mechanical and thermal stabilities, and moisture barrier properties, which are the essential characteristics for active antibacterial packaging films. The PCs have been studied in a number of applications by direct contact with foods and beverages; however, they have very poor antibacterial activities, which reduce their efficiency in antibacterial packaging system effectively. The antibacterial activities of the PC have been enhanced by functionalizing reactive groups/blending with antibacterial agents [7–9].In this research, we have reported leaf extract incorporated PC films, which were fabricated using solution blending followed by Thermally Induced Phase Separation technique. Here, the maceration was employed for preparing the leaf extract, in which the solvents diffuse into the solid plant material and solubilize their compounds. The as-prepared leaf extracts are safe and effective for long term use, since they possess antibacterial molecules as well as antioxidants. The following medicinal leaves crude extracts were used in this study. Firstly, the extract that was collected from the leaf ofAzadirachta indica (neem) has flavonoids, dihydrochalcones, arabinogalactans, isoprenoids, polyphenolics, coumarin, and tannins, which are the important constituents for its antibacterial activities [10]. Then,Psidium guajava (Guava) leaf extract consists of effective phytochemical constituents such as acalypus, tannins, saponins, and acalyphine for its antibacterial nature [11].Acalypha indica, commonly known as Indian Acalypha, has potential antibacterial molecules such as acalyphine, cyanogenic glucosides, alkaloids, and triacetone amine. Furthermore, the leaf extract ofAndrographis paniculata (Green Chiretta) contains flavonoids, alkaloids, steroids, phenols, tannins, and particularly andrographolide for its antibacterial efficacy [12]. Finally, the fresh leaf ofOcimum sanctum (Holy Basil) possesses steroid, flavonoid, phenols, tannin, alkaloid, saponin, and carotenoid compounds, and it could be also used as insecticide, antibiotics, and fungicide [13]. All the leaf extracts possess the vital properties like antifungal, antiviral, antioxidant, anti-inflammatory, and antipyretic. Based on the above merits, the mentioned leaf extract was prepared by maceration for blending with the PC solution to obtain active antibacterial thin films.Here, we report a facile, low-cost, and scalable technique for the fabrication of PC/LE films. In addition, the antibacterial activities of the PC and PC/LE films were assessed againstS. aureus andE. coli, which are identified as food spoilage bacteria. To the best of our knowledge, in an open literature, the antibacterial studies of mentioned crude leaf extract incorporated PC thin films have not yet been reported for active antibacterial packaging applications.


## 2. Materials and Methods

### 2.1. Materials

Bisphenol A polycarbonate (PC;Mw~1,50,000 g/mol molecular weight of repeating unit: 254.3 g/mol; polydispersity index: 1.8) was supplied by GE Plastic, Ltd., India, and dried at 100°C in an oven for 6 hrs prior to use.Azadirachta indica, Psidium guajava, Acalypha indica, Andrographis paniculata, andOcimum sanctum were collected at various regions, which were mentioned in Table 1.Prunus (plum), fruit model, were cleaned with distilled water several times to remove the adhering impurities on the surface. N,N-Dimethylformamide (DMF) was purchased from Sigma-Aldrich, India, and used as received. The list of abbreviations of the chemicals and leaves used in this study is listed in Abbreviations.Table 1
Descriptive features of the leaf used for the antibacterial assay.
S. number Botanical species Family name Location(DMS latitude) Studied organ 1 Acalypha indica Myrtaceae N 10°47′13′′ Leaves 2 Psidium guajava Euphorbiaceae N 10°46′19′′ Leaves 3 Andrographis paniculata Acanthaceae N 10°39′36′′ Leaves 4 Ocimum sanctum Lamiaceae N 10°46′19′′ Leaves 5 Azadirachta indica Meliaceae N 10°39′36′′ Leaves


### 2.2. Processing of the Leaf

Firstly, the leaves (Azadirachta indica, Psidium guajava, Acalypha indica, Andrographis paniculata, andOcimum sanctum) were washed with running tap water for 15 min, followed by distilled water several times to remove the impurities on the leaves’ surface. The samples were dried at room temperature under shade for 10 days to evaporate the residual water. The leaves were finely ground by stainless steel grinder to turn them to powdery form and stored in airtight containers [14, 15].


### 2.3. Preparation of Leaf Extract

Powdered leaf (10 g) was poured in an Erlenmeyer flask containing 100 mL of DMF. The flask was put on a hot plate for 10 min and kept aside for 24 h at room temperature for complete maceration. Then, the macerate was filtered through nylon mesh followed by Whatman number 1 filter paper. The similar procedure was followed by preparing all the leaf crude extracts. In addition, for the preparation of PC-AI 2 and PC-AI 3 samples, 20 g and 30 g of dried neem powder were macerated in DMF (100 mL), respectively [16].


### 2.4. Fabrication of PC and PC/LE Films

The PC and PC/LE thin films were fabricated by solution blending followed by TIPS [17, 18]. Figure 1 shows the schematic representation of the fabrication of PC/LE thin films. The figure reveals the processing of neem leaves, maceration of the neem powder, and the appearance of as-prepared film with inhibition zones, respectively. Briefly, the PC (15 wt%) was dissolved in DMF and stirred for 5 hrs by magnetic stirring to obtain a homogeneous solution. Consequently, the as-prepared leaf extract (10 mL) was added to the PC solution, with stirring for 5 hrs at room temperature. The PC/LE solution was poured on a glass plate and cast by a doctor blade (thickness 50 μm) at room temperature. The nascent film was being kept on a hot plate (80°C) to evaporate the solvent. Then, the film was peeled off and placed in a stainless steel plate at 100°C for 2 hr to remove the residual solvent completely. The thickness of the as-prepared films was measured using a digital micrometer (Mitutoyo, Tokyo, Japan), at different locations and an average value of six measurements was taken for each film.Figure 1
Schematic representation of fabrication of PC/LE thin films.


### 2.5. Fruit Model Studies

The antibacterial efficacy of the PC and PC/LE films was assessed usinggenus Prunus as a model fruit. FreshPrunus of almost equal size were washed with distilled water and then dried at room temperature for 3 hrs.Prunus was wrapped with the as-prepared films individually and placed in an open atmosphere, and the unwrappedPrunus was served as control [19].


### 2.6. Evaluation of Antibacterial Activity

The antibacterial activities of the PC and PC/LE films were assessed usingE. coli (Gram-negative, ATCC 25922) andS. aureus (Gram-positive, ATCC29213) by Disc Diffusion method (Kirby Bauer test) [20, 21]. Briefly, the sterilized Mueller-Hinton agar was poured in Petri plates; after solidification, the inoculums were spread on the plate using L-rod. Later, the as-prepared films were cut into pieces and placed on the bacterial strain. The plates were incubated for 24 h in an aerobic incubation chamber. The inhibition zones around the films were visually identified and the diameter of the inhibition zone was also measured.


## 2.1. Materials

Bisphenol A polycarbonate (PC;Mw~1,50,000 g/mol molecular weight of repeating unit: 254.3 g/mol; polydispersity index: 1.8) was supplied by GE Plastic, Ltd., India, and dried at 100°C in an oven for 6 hrs prior to use.Azadirachta indica, Psidium guajava, Acalypha indica, Andrographis paniculata, andOcimum sanctum were collected at various regions, which were mentioned in Table 1.Prunus (plum), fruit model, were cleaned with distilled water several times to remove the adhering impurities on the surface. N,N-Dimethylformamide (DMF) was purchased from Sigma-Aldrich, India, and used as received. The list of abbreviations of the chemicals and leaves used in this study is listed in Abbreviations.Table 1
Descriptive features of the leaf used for the antibacterial assay.
S. number Botanical species Family name Location(DMS latitude) Studied organ 1 Acalypha indica Myrtaceae N 10°47′13′′ Leaves 2 Psidium guajava Euphorbiaceae N 10°46′19′′ Leaves 3 Andrographis paniculata Acanthaceae N 10°39′36′′ Leaves 4 Ocimum sanctum Lamiaceae N 10°46′19′′ Leaves 5 Azadirachta indica Meliaceae N 10°39′36′′ Leaves


## 2.2. Processing of the Leaf

Firstly, the leaves (Azadirachta indica, Psidium guajava, Acalypha indica, Andrographis paniculata, andOcimum sanctum) were washed with running tap water for 15 min, followed by distilled water several times to remove the impurities on the leaves’ surface. The samples were dried at room temperature under shade for 10 days to evaporate the residual water. The leaves were finely ground by stainless steel grinder to turn them to powdery form and stored in airtight containers [14, 15].


## 2.3. Preparation of Leaf Extract

Powdered leaf (10 g) was poured in an Erlenmeyer flask containing 100 mL of DMF. The flask was put on a hot plate for 10 min and kept aside for 24 h at room temperature for complete maceration. Then, the macerate was filtered through nylon mesh followed by Whatman number 1 filter paper. The similar procedure was followed by preparing all the leaf crude extracts. In addition, for the preparation of PC-AI 2 and PC-AI 3 samples, 20 g and 30 g of dried neem powder were macerated in DMF (100 mL), respectively [16].


## 2.4. Fabrication of PC and PC/LE Films

The PC and PC/LE thin films were fabricated by solution blending followed by TIPS [17, 18]. Figure 1 shows the schematic representation of the fabrication of PC/LE thin films. The figure reveals the processing of neem leaves, maceration of the neem powder, and the appearance of as-prepared film with inhibition zones, respectively. Briefly, the PC (15 wt%) was dissolved in DMF and stirred for 5 hrs by magnetic stirring to obtain a homogeneous solution. Consequently, the as-prepared leaf extract (10 mL) was added to the PC solution, with stirring for 5 hrs at room temperature. The PC/LE solution was poured on a glass plate and cast by a doctor blade (thickness 50 μm) at room temperature. The nascent film was being kept on a hot plate (80°C) to evaporate the solvent. Then, the film was peeled off and placed in a stainless steel plate at 100°C for 2 hr to remove the residual solvent completely. The thickness of the as-prepared films was measured using a digital micrometer (Mitutoyo, Tokyo, Japan), at different locations and an average value of six measurements was taken for each film.Figure 1
Schematic representation of fabrication of PC/LE thin films.


## 2.5. Fruit Model Studies

The antibacterial efficacy of the PC and PC/LE films was assessed usinggenus Prunus as a model fruit. FreshPrunus of almost equal size were washed with distilled water and then dried at room temperature for 3 hrs.Prunus was wrapped with the as-prepared films individually and placed in an open atmosphere, and the unwrappedPrunus was served as control [19].


## 2.6. Evaluation of Antibacterial Activity

The antibacterial activities of the PC and PC/LE films were assessed usingE. coli (Gram-negative, ATCC 25922) andS. aureus (Gram-positive, ATCC29213) by Disc Diffusion method (Kirby Bauer test) [20, 21]. Briefly, the sterilized Mueller-Hinton agar was poured in Petri plates; after solidification, the inoculums were spread on the plate using L-rod. Later, the as-prepared films were cut into pieces and placed on the bacterial strain. The plates were incubated for 24 h in an aerobic incubation chamber. The inhibition zones around the films were visually identified and the diameter of the inhibition zone was also measured.


## 3. Results and Discussion

Table2 shows the PC/LE weight ratio and thickness of the as-prepared thin films. The thickness of the PC-AI 1, PC-AI 2, and PC-AI 3 thin films minutely increased with respect to the concentration of neem leaf extract in the PC matrix, and the thickness of the remaining films did not change significantly. Figure 2 shows the PC, PC-AC, PC-PG, PC-OS, PC-AI 1, PC-AI 2, and PC-AI 3 transparent thin films on the flower image; the color of the films shifted from dull to dark greenish with respect to the chlorophyll and other constituents in content of the leaf extract [22]. The pristine PC film appears transparent and colorless, which is shown in Figure 2. However, the PC-AC, PC-PG, and PC-OS films have light greenish color, due to low content of chlorophyll in their leaf. Since the content of neem leaf extract increased from 10 to 30 wt%, the color of the resulting films changed from light green (PC-AI 1) to dark green (PC-AI 3). At higher quantity (40 mL) ofAzadirachta indica leaf extract in the polymer matrix, the film lost its transparency slightly, and the leaf extract did not homogeneously mix within the matrix.Table 2
Composition and thickness of as-prepared PC and PC/LE thin films.
S. number Thin film code PC(wt%) Leaves extract(mL) Thickness(µm) 1 PC 30 10 17 2 PC-AC 30 10 25 3 PC-PG 30 10 24 4 PC-AP 30 10 23 5 PC-OS 30 10 26 6 PC-AI 1 30 10 27 7 PC-AI 2 30 20 29 8 PC-AI 3 30 30 30Figure 2
Photographic images of PC and PC/LE thin films.Figure3 shows photographic images of the model fruit sample ofPrunus, unwrapped control and wrapped with pristine PC and PC/LE films. The preservation study had been carried out for 11 days, until the control and PC wrappedPrunus spoiled. After 11 days,Prunus wrapped with the PC/LE films retained higher shelf-life and freshness, compared with the control and PC wrapped one. In these fruit model studies, the control sample started to deteriorate after 3 days, and the PC wrapped sample deteriorated after 5 days. From the images (Figure 3), it can be concluded thatPrunus (control) andPrunus covered with pristine PC film started to damage and deteriorate due to the attack of bacterial pathogens, whereasPrunus wrapped with the PC/LE films maintained freshness and the shape of the fruit, even after 11 days of storage time due to their antibacterial characteristics [23].Figure 3
Photographic images ofPrunus (a), pristine PC (b), PC-AC (c), PC-PG (d), PC-OS (e), and PC-AI 1 (f). After 11 days,Prunus (g), pristine PC (h), PC-AC (i), PC-PG (j), PC-OS (k), and PC-AI 1 (l).
(a) (b) (c) (d) (e) (f) (g) (h) (i) (j) (k) (l)Figure4 shows photographic images of PC and PC/LE films on the bacterial lawn. The pristine PC films did not show any significant inhibition zone for both bacteria, whereas the PC/LE films were more effective and exhibited inhibition zones forE. coli andS. aureus. This is due to the presence of antibacterial agents in the leaf extracts, which did effectively function in the PC matrix. In this research, all the PC/LE films possessed significant inhibitory activities againstE. coli andS. aureus, which concluded that the leaf extracts also retain their antibacterial property in the polymer matrix.Figure 4
Inhibition zones of films againstE. coli (a and b) andS. aureus (c and d): PC (1), PC-AC (2), PC-PG (3), PC-AP (4), PC-OS (5), PC-AI 1 (6), PC-AI 2 (7), and PC-AI 3 (8).
(a) (b) (c) (d)In Figure5, the PC-OS sample showed the highest inhibition zones of 8.21 and 7.82 mm forE. coli andS. aureus, respectively, due to the presence of effective antibacterial agents such as saponins, alkaloids, flavonoids, cardiac glycosides, steroids, phenols, and tannin [24]. In the PC-AI 1–3 films, since the leaf extract concentration was increased from 10 mL to 30 mL, the antibacterial activity of the films also was significantly enhanced, meaning that the bacteria have been killed faster at higher concentration of antibacterial agents in the PC films [25]. The antibacterial studies revealed that the efficacy of the antibacterial agents againstS. aureus was higher for all the films compared withE. coli. This might be due to the fact that the damage of cell wall structure of theS. aureus is easier than theE. coli by bactericidal molecules in the leaf extract. ForE. coli, the PC-AC, PC-PG, PC-AP, PC-OS, PC-AI 1, and PC-AI 2 exhibited the inhibition zones of 3.24, 2.13, 3.32, 8.12, 1.32, and 4.51 mm, respectively. In case ofS. aureus, the inhibition zones were observed around 3.43, 3.30, 5.43, 7.64, 1.16, 4.21, and 6.48 mm for the PC-AC, PC-PG, PC-AP, PC-OS, PC-AI 1, and PC-AI 2, respectively. The results concluded that the antibacterial agents present in the leaf effectively destroyed theS. aureus more than theE. coli.Figure 5
Comparison of antibacterial activities of PC and PC/LE films againstE. coli andS. aureus.


## 4. Conclusion

A simple and reliable route has been proposed to fabricate bactericidal films by incorporating leaf extract into the polymer matrix. The as-prepared films showed significant antibacterial activities againstE. coli andS. aureus. Specifically,P. guajava based PC thin films exhibited the highest antibacterial activities against both bacteria even at low loading (10 wt%) of leaf extract in the polymer matrix. Most of the films showed excellent inhibitory effects againstS. aureus compared to theE. coli. More importantly, the model fruit studies revealed that the as-prepared PC/LE films could be the promising materials in antibacterial packaging applications due to their significant antibacterial efficacy.



---

*Source: 3194154-2016-10-09.xml*